# Two dimensional correlation spectroscopy applications in vibratioal and optical spectroscopy - Isao N.

ISBN 0-471-62391-1

**Download**(direct link)

**:**

**85**> 86 87 88 89 90 91 .. 120 >> Next

Composition-based 2D Raman Study of EVA Copolymers 205

Table 10.2 Assignments of the Raman bands of EVA (from Ref. No. 24)

Frequency (cm-1) Mode Features“

629 O-C=O deformation Due to acetate

647 O-C=O deformation Due to acetate

1018 C-C stretching of >HC-CH2 Due to vinyl

1060 asymmetric C-C stretching Due to all-trans -(CH2)-„

1079 asymmetric C-C stretching A (trans and gauche)

1110 symmetric C-C stretching A (trans and gauche)

1130 symmetric C-C stretching Due to all-trans -(CH2)-„

1172 CH2 rocking C

1295 CH2 twisting Due to all-trans -(CH2)-„

1307 CH2 twisting A

1330 CH2 wagging A

1349 CH2 wagging A

1373 CH2 wagging A

1380 CH3 symmetric bending Due to acetate

1415 CH2 bending C

1430 CH3 asymmetric bending Due to acetate

1434 CH2 bending N

1438 CH2 bending C

1446 CH2 bending N

1461 2 x CH2 rocking Due to all-trans -(CH2)-„

1739 C=O stretching Due to acetate

aA, amorphous; C, crystalline; N, anisotropic.

level, the spectral data were subdivided into four distinct sets according to their composition range.

Set 1 contained three EVA copolymers with low VA content of 6, 7 and 8 wt%. Synchronous and asynchronous correlation spectra for Set 1 in the region 1500-1200 cm-1 are shown in Figure 10.21(A) and (B).24 A band at 1415 cm-1 is ascribed to the lamellar cores that constitute the orthorhombic crystalline phase, while that at 1307 cm-1 is attributed to the interlamellar layers that make up the amorphous phase.41 The negative synchronous cross peak at (1415, 1307 cm-1) indicates that the intensity of the crystalline band at 1415 cm-1 decreases, while that of the amorphous band at 1307 cm-1 increases. Thus, the crystalline lamellae shrink, and the interlamellar amorphous layers expand with a small increase in VA content.

In the synchronous spectrum, bands at 1446 and 1434 cm-1 have negative correlation with the crystalline band at 1415 cm-1 and positive correlation with each other. The band at 1446 cm-1 has positive correlation with the amorphous band at 1307 cm-1. These observations suggest the intensity changes of the bands at 1446 and 1434 cm-1 have the same direction as the amorphous band at 1307 cm-1, and opposite direction with respect to the crystalline band at 1415 cm-1. However, it is not enough to conclude that the two bands at 1446 and 1434 cm-1 arise from the amorphous phase. Note that they share asynchronous cross peaks with the

206

Generalized 2D Correlation Studies of Polymers and Liquid Crystals

(A)

(B)

Wavenumber/cm-1, v1 Wavenumber/cm 1, v1

Figure 10.21 (A) Synchronous 2D Raman correlation spectrum in the 1500-1200 cm-1

region for EVA copolymers with VA from 6 to 8wt%. (B) The corresponding asynchronous correlation spectrum. (Reproduced with permission from Ref. No. 24. Copyright (1999) American Chemical Society.)

amorphous band at 1307 cm-1 (Figure 10.21(B)). Therefore, it is very likely that these bands arise from an anisotropic phase. This phase is believed to exist as transition layer between the lamella and interlamellar amorphous layers.41 However, this anisotropic layer is not quite like that originally proposed by Strobl and Hagedorn,41 which does not have any lateral order. Ren et at.24 concluded that the acetate side groups act as spacers between adjacent chains and reduce the interaction force between their hydrogen atoms, and hence the magnitude of correlation splittings.42 The bands at 1446 and 1434 cm-1 are thus assigned to the correlation splittings of CH2 bending vibrations in the anisotropic phase. The splitting is only 8 cm-1, considerably smaller than the 23 cm-1 splitting between 1438 and 1415 cm-1 in the crystalline phase.

The order of intensity changes between two bands is listed in Table 10.3.24 From the first and second rows of Table 10.3, it is concluded that the intensity variations of bands at 1446 and 1434 cm-1 take place before (i.e., at a lower VA content) that of the band at 1307 cm-1. Thus, for Set 1 the inclusion of a VA comonomer first causes the expansion of the anisotropic phase, then the expansion of the amorphous phase. The physical implication here is that the acetate side groups act as spacers between adjacent chains, thereby converting the tightly packed orthorhombic phase to the loosely packed anisotropic phase. The anisotropic phase then transforms to the amorphous phase.

Figure 10.22 illustrates a synchronous correlation spectrum for Set 1 in the regions 1500-1200 cm-1 and 1200-1000 cm-1.24 Bands at 1130 and 1060 cm-1 are due, respectively, to antisymmetric and symmetric C-C stretching vibrations of all-tranv chains of CH3(CH2)nCH3 for n > 6.43 These bands should be highly overlapped, since they come from both the anisotropic phase and the

Composition-based 2D Raman Study of EVA Copolymers

207

Table 10.3 Synchronous and asynchronous correlation intensities and the order of intensity change between two bands“ (from Ref. 24)

Number $ Order

1 $ 1446, 1307) > 0 ^ (1446, 1307) > 0 1446 cm before 1307 cm-1

**85**> 86 87 88 89 90 91 .. 120 >> Next